LMucko/crystallography-open-database huggingface dataset:
Phase equilibria in the Lu - V - B system and the structure of the new boride Lu1.34 V1.66 B6
Mikhalenko, S.I.; Chaban, N.F.; Kuz'ma, Yu.B.; Davidov, V.M.; Powder Metallurgy and Metal Ceramics 41 (2002) 162–168; doi:10.1023/A:1019887027364

data_1510748
_publ_section_title
;
 Phase equilibria in the Lu - V - B system and the structure of the new
 boride Lu1.34 V1.66 B6
;
_journal_name_full               'Powder Metallurgy and Metal Ceramics'
_journal_page_first              162
_journal_page_last               168
_journal_paper_doi               10.1023/A:1019887027364
_journal_volume                  41
_journal_year                    2002
_chemical_formula_sum            'B2 Lu0.95 V0.05'
_chemical_name_systematic        '(Lu0.95 V0.05) B2'
_space_group_IT_number           191
_symmetry_space_group_name_Hall  '-P 6 2'
_symmetry_space_group_name_H-M   'P 6/m m m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            1
_cell_length_a                   3.238
_cell_length_b                   3.238
_cell_length_c                   3.689
_cell_volume                     33.496
_citation_journal_id_ASTM        PMMCEF
_cod_data_source_file            boron_239.cif
_cod_data_source_block           B2Lu0.95V0.05
_cod_database_code               1510748
Bismuth borates: One-dimensional borate chains and nonlinear optical properties
Li, G.; Lin, J.; Wang, Y.; Li, L.; Liao, F.; Chemistry of Materials (1,1989-) 17 (2005) 4174–4180; doi:

data_4001736
_publ_section_title
;
 Bismuth borates: One-dimensional borate chains and nonlinear optical
 properties
;
_journal_name_full               'Chemistry of Materials (1,1989-)'
_journal_page_first              4174
_journal_page_last               4180
_journal_volume                  17
_journal_year                    2005
_chemical_formula_sum            'B2 Bi F O4'
_chemical_name_systematic        'Bi B2 O4 F'
_space_group_IT_number           145
_symmetry_space_group_name_Hall  'P 32'
_symmetry_space_group_name_H-M   'P 32'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            3
_cell_length_a                   6.7147
_cell_length_b                   6.7147
_cell_length_c                   6.4688
_cell_volume                     252.585
_citation_journal_id_ASTM        CMATEX
_cod_data_source_file            boron_24.cif
_cod_data_source_block           B2Bi1F1O4
_cod_original_formula_sum        'B2 Bi1 F1 O4'
_cod_database_code               4001736
Phase relations in the ternary systems rare.earth metal (RE)-boron-nitrogen, where RE= Tb, Dy, Ho, Er, Tm, Lu, Sc and Y
Rogl, P.; Klesnar, H.P.; High Temperatures-High Pressures 22 (1990) 453–457; doi:

data_1510749
_publ_section_title
;
 Phase relations in the ternary systems rare.earth metal
 (RE)-boron-nitrogen, where RE= Tb, Dy, Ho, Er, Tm, Lu, Sc and Y
;
_journal_name_full               'High Temperatures-High Pressures'
_journal_page_first              453
_journal_page_last               457
_journal_volume                  22
_journal_year                    1990
_chemical_formula_sum            'B2 Lu'
_chemical_name_systematic        'Lu B2'
_space_group_IT_number           191
_symmetry_space_group_name_Hall  '-P 6 2'
_symmetry_space_group_name_H-M   'P 6/m m m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            1
_cell_length_a                   3.2442
_cell_length_b                   3.2442
_cell_length_c                   3.7061
_cell_volume                     33.780
_citation_journal_id_ASTM        HTHPAK
_cod_data_source_file            boron_240.cif
_cod_data_source_block           B2Lu1
_cod_original_cell_volume        33.78026
_cod_original_formula_sum        'B2 Lu1'
_cod_database_code               1510749
Comparitive critical field study of superconducting ternary borides
Lee, W.H.; Appl, S.; Shelton, R.N.; Journal of Low Temperature Physics 68 (1987) 147–157; doi:10.1007/BF00682626

data_1510750
_publ_section_title
;
 Comparitive critical field study of superconducting ternary borides
;
_journal_name_full               'Journal of Low Temperature Physics'
_journal_page_first              147
_journal_page_last               157
_journal_paper_doi               10.1007/BF00682626
_journal_volume                  68
_journal_year                    1987
_chemical_formula_sum            'B2 Lu Os3'
_chemical_name_systematic        'Lu Os3 B2'
_space_group_IT_number           191
_symmetry_space_group_name_Hall  '-P 6 2'
_symmetry_space_group_name_H-M   'P 6/m m m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            1
_cell_length_a                   5.455
_cell_length_b                   5.455
_cell_length_c                   3.064
_cell_volume                     78.960
_citation_journal_id_ASTM        JLTPAC
_cod_data_source_file            boron_241.cif
_cod_data_source_block           B2Lu1Os3
_cod_original_cell_volume        78.96031
_cod_original_formula_sum        'B2 Lu1 Os3'
_cod_database_code               1510750
Crystal structure of Lu Ru B2
Ku, H.C.; Shelton, R.N.; Materials Research Bulletin 15 (1980) 1445–1452; doi:10.1016/0025-5408(80)90100-2

data_1510751
_publ_section_title
;
 Crystal structure of Lu Ru B2
;
_journal_name_full               'Materials Research Bulletin'
_journal_page_first              1445
_journal_page_last               1452
_journal_paper_doi               10.1016/0025-5408(80)90100-2
_journal_volume                  15
_journal_year                    1980
_chemical_formula_sum            'B2 Lu Ru'
_chemical_name_systematic        'Lu Ru B2'
_space_group_IT_number           62
_symmetry_space_group_name_Hall  '-P 2ac 2n'
_symmetry_space_group_name_H-M   'P n m a'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   5.809
_cell_length_b                   5.229
_cell_length_c                   6.284
_cell_volume                     190.878
_citation_journal_id_ASTM        MRBUAC
_cod_data_source_file            boron_242.cif
_cod_data_source_block           B2Lu1Ru1
_cod_original_cell_volume        190.8781
_cod_original_formula_sum        'B2 Lu1 Ru1'
_cod_database_code               1510751
Magnetic behavior and structural chemistry of RE Ru3 B2 borides
Hiebl, K.; Uhl, E.; Sienko, M.J.; Rogl, P.; Inorganic Chemistry 19 (1980) 3316–3320; doi:10.1021/ic50213a022

data_4331427
_publ_section_title
;
 Magnetic behavior and structural chemistry of RE Ru3 B2 borides
;
_journal_name_full               'Inorganic Chemistry'
_journal_page_first              3316
_journal_page_last               3320
_journal_paper_doi               10.1021/ic50213a022
_journal_volume                  19
_journal_year                    1980
_chemical_formula_sum            'B2 Lu Ru3'
_chemical_name_systematic        'Lu Ru3 B2'
_space_group_IT_number           191
_symmetry_space_group_name_Hall  '-P 6 2'
_symmetry_space_group_name_H-M   'P 6/m m m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            1
_cell_length_a                   5.439
_cell_length_b                   5.439
_cell_length_c                   3.016
_cell_volume                     77.268
_citation_journal_id_ASTM        INOCAJ
_cod_data_source_file            boron_243.cif
_cod_data_source_block           B2Lu1Ru3
_cod_original_cell_volume        77.26808
_cod_original_formula_sum        'B2 Lu1 Ru3'
_cod_database_code               4331427
Synthese und Kristallstruktur von manganhaltigen Pyroboraten: Mn Co (B2 O5) und Mn Mg (B2 O5)
Bluhm, K.; Utzolino, A.; Zeitschrift fuer Naturforschung, Teil B. Anorganische Chemie, Organische Chemie (42,1987-) 51 (1996) 912–916; doi:

data_7209436
_publ_section_title
;
 Synthese und Kristallstruktur von manganhaltigen Pyroboraten: Mn Co (B2
 O5) und Mn Mg (B2 O5)
;
_journal_name_full
;
Zeitschrift fuer Naturforschung, Teil B. Anorganische Chemie, Organische
 Chemie (42,1987-)
;
_journal_page_first              912
_journal_page_last               916
_journal_volume                  51
_journal_year                    1996
_chemical_formula_sum            'B2 Mg Mn O5'
_chemical_name_systematic        'Mn Mg (B2 O5)'
_space_group_IT_number           2
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_cell_angle_alpha                104.47
_cell_angle_beta                 90.6
_cell_angle_gamma                91.98
_cell_formula_units_Z            2
_cell_length_a                   3.1897
_cell_length_b                   6.198
_cell_length_c                   9.367
_cell_volume                     179.167
_citation_journal_id_ASTM        ZNBSEN
_cod_data_source_file            boron_244.cif
_cod_data_source_block           B2Mg1Mn1O5
_cod_original_cell_volume        179.1671
_cod_original_formula_sum        'B2 Mg1 Mn1 O5'
_cod_database_code               7209436
Darstellung und Kristallstruktur von Mg Ni2.5 B2 und Li1.2 Ni2.5 B2
Jung, W.; Zeitschrift fuer Naturforschung, Teil B. Anorganische Chemie, Organische Chemie (2,1947-32,1977) 32 (1977) 1371–1374; doi:

data_7209437
_publ_section_title
;
 Darstellung und Kristallstruktur von Mg Ni2.5 B2 und Li1.2 Ni2.5 B2
;
_journal_name_full
;
Zeitschrift fuer Naturforschung, Teil B. Anorganische Chemie, Organische
 Chemie (2,1947-32,1977)
;
_journal_page_first              1371
_journal_page_last               1374
_journal_volume                  32
_journal_year                    1977
_chemical_formula_sum            'B2 Mg Ni2.5'
_chemical_name_systematic        'Mg Ni2.5 B2'
_space_group_IT_number           180
_symmetry_space_group_name_Hall  'P 62 2 (0 0 4)'
_symmetry_space_group_name_H-M   'P 62 2 2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            3
_cell_length_a                   4.887
_cell_length_b                   4.887
_cell_length_c                   8.789
_cell_volume                     181.784
_citation_journal_id_ASTM        ZENBAX
_cod_data_source_file            boron_245.cif
_cod_data_source_block           B2Mg1Ni2.5
_cod_original_cell_volume        181.7836
_cod_original_sg_symbol_Hall     'P 62 2 (x,y,z+1/3)'
_cod_original_formula_sum        'B2 Mg1 Ni2.5'
_cod_database_code               7209437
Die Struktur der ternaeren Boride vom Chromkarbid -C23 C6-Typ
Stadelmaier, H.H.; Draughn, R.A.; Hofer, G.; Zeitschrift fuer Metallkunde 54 (1963) 640–644; doi:

data_1510752
_publ_section_title
;
 Die Struktur der ternaeren Boride vom Chromkarbid -C23 C6-Typ
;
_journal_name_full               'Zeitschrift fuer Metallkunde'
_journal_page_first              640
_journal_page_last               644
_journal_volume                  54
_journal_year                    1963
_chemical_formula_sum            'B2 Mg Ni6.7'
_chemical_name_systematic        'Mg Ni6.7 B2'
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            12
_cell_length_a                   10.569
_cell_length_b                   10.569
_cell_length_c                   10.569
_cell_volume                     1180.597
_citation_journal_id_ASTM        ZEMTAE
_cod_data_source_file            boron_246.cif
_cod_data_source_block           B2Mg1Ni6.7
_cod_original_formula_sum        'B2 Mg1 Ni6.7'
_cod_database_code               1510752
Borates Me(IV) Me(II) (B O3)2 de structure dolomite
Vicat, J.; Aleonard, S.; Comptes Rendus Hebdomadaires des Seances de l'Academie des Sciences, Serie C, Sciences Chimiques (1966-) 266 (1968) 1046–1049; doi:

data_1510753
_publ_section_title
;
 Borates Me(IV) Me(II) (B O3)2 de structure dolomite
;
_journal_name_full
;
Comptes Rendus Hebdomadaires des Seances de l'Academie des Sciences, Serie C,
 Sciences Chimiques (1966-)
;
_journal_page_first              1046
_journal_page_last               1049
_journal_volume                  266
_journal_year                    1968
_chemical_formula_sum            'B2 Mg O6 Sn'
_chemical_name_systematic        'Mg Sn (B O3)2'
_space_group_IT_number           148
_symmetry_space_group_name_Hall  '-R 3'
_symmetry_space_group_name_H-M   'R -3 :H'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            3
_cell_length_a                   4.707
_cell_length_b                   4.707
_cell_length_c                   14.93
_cell_volume                     286.470
_citation_journal_id_ASTM        CHDCAQ
_cod_data_source_file            boron_247.cif
_cod_data_source_block           B2Mg1O6Sn1
_cod_original_cell_volume        286.4698
_cod_original_formula_sum        'B2 Mg1 O6 Sn1'
_cod_database_code               1510753
Ternary rhodium borides A3 Rh5 B2 (A = Mg, Sc) and quaternary derivates A2 M Rh5 B2. Preparation, crystal structure (M = main group and 3 d elements), and magnetism (M = Mn, Fe)
Lueken, H.; Mueller, P.; Nagelschmitz, E.A.; Feiten, R.; Jung, W.; Zeitschrift fuer Anorganische und Allgemeine Chemie 627 (2001) 523–532; doi:10.1002/1521-3749(200103)627:3<523::AID-ZAAC523>3.0.CO;2-E

data_1510754
_publ_section_title
;
 Ternary rhodium borides A3 Rh5 B2 (A = Mg, Sc) and quaternary derivates
 A2 M Rh5 B2. Preparation, crystal structure (M = main group and 3 d
 elements), and magnetism (M = Mn, Fe)
;
_journal_name_full
'Zeitschrift fuer Anorganische und Allgemeine Chemie'
_journal_page_first              523
_journal_page_last               532
_journal_paper_doi
10.1002/1521-3749(200103)627:3<523::AID-ZAAC523>3.0.CO;2-E
_journal_volume                  627
_journal_year                    2001
_chemical_formula_sum            'B2 Mg2 P0.92 Rh5'
_chemical_name_systematic        'Mg2 P0.92 Rh5 B2'
_space_group_IT_number           127
_symmetry_space_group_name_Hall  '-P 4 2ab'
_symmetry_space_group_name_H-M   'P 4/m b m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   9.239
_cell_length_b                   9.239
_cell_length_c                   2.896
_cell_volume                     247.200
_citation_journal_id_ASTM        ZAACAB
_cod_data_source_file            boron_248.cif
_cod_data_source_block           B2Mg2P0.92Rh5
_cod_original_cell_volume        247.2
_cod_database_code               1510754
The crystal structures of warwickite, ludwigite and pinakiolite
Watanabe, T.; Ito, T.; Takeuchi, Y.; Acta Crystallographica (1,1948-23,1967) 3 (1950) 98–107; doi:10.1107/S0365110X50000252

data_2310088
_publ_section_title
;
 The crystal structures of warwickite, ludwigite and pinakiolite
;
_journal_name_full               'Acta Crystallographica (1,1948-23,1967)'
_journal_page_first              98
_journal_page_last               107
_journal_paper_doi               10.1107/S0365110X50000252
_journal_volume                  3
_journal_year                    1950
_chemical_formula_sum            'B2 Mg3 Mn3 O10'
_chemical_name_systematic        'Mg3 Mn3 (B2 O10)'
_space_group_IT_number           11
_symmetry_space_group_name_Hall  '-P 2yb'
_symmetry_space_group_name_H-M   'P 1 21/m 1'
_cell_angle_alpha                90
_cell_angle_beta                 120.57
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   5.36
_cell_length_b                   5.98
_cell_length_c                   12.73
_cell_volume                     351.319
_citation_journal_id_ASTM        ACCRA9
_cod_data_source_file            boron_249.cif
_cod_data_source_block           B2Mg3Mn3O10
_cod_original_cell_volume        351.3191
_cod_database_code               2310088
The crystal structure of bismuth (2/1) borate, (Bi2 O3 B2 O3)2
Perloff, A.; Hyman, A.; Acta Crystallographica B (24,1968-38,1982) 28 (1972) 2007–2011; doi:10.1107/S0567740872005436

data_2105402
_publ_section_title
;
 The crystal structure of bismuth (2/1) borate, (Bi2 O3 B2 O3)2
;
_journal_name_full               'Acta Crystallographica B (24,1968-38,1982)'
_journal_page_first              2007
_journal_page_last               2011
_journal_paper_doi               10.1107/S0567740872005436
_journal_volume                  28
_journal_year                    1972
_chemical_formula_sum            'B2 Bi4 O9'
_chemical_name_systematic        'Bi4 B2 O9'
_space_group_IT_number           14
_symmetry_space_group_name_Hall  '-P 2ybc'
_symmetry_space_group_name_H-M   'P 1 21/c 1'
_cell_angle_alpha                90
_cell_angle_beta                 91.04
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   11.107
_cell_length_b                   6.627
_cell_length_c                   11.044
_cell_volume                     812.772
_citation_journal_id_ASTM        ACBCAR
_cod_data_source_file            boron_25.cif
_cod_data_source_block           B2Bi4O9
_cod_original_cell_volume        812.7717
_cod_database_code               2105402
Phase equilibria in the systems vanadium-manganese-boron, molybdenum-manganese-boron, and tungsten-manganese-boron
Telegus, V.S.; Kuz'ma, Yu.B.; Poroshkovaya Metallurgiya 10 (1971) 52–56; doi:

data_1510755
_publ_section_title
;
 Phase equilibria in the systems vanadium-manganese-boron,
 molybdenum-manganese-boron, and tungsten-manganese-boron
;
_journal_name_full               'Poroshkovaya Metallurgiya'
_journal_page_first              52
_journal_page_last               56
_journal_volume                  10
_journal_year                    1971
_chemical_formula_sum            'B2 Mn0.64 Mo0.36'
_chemical_name_systematic        '(Mn0.64 Mo0.36) B2'
_space_group_IT_number           191
_symmetry_space_group_name_Hall  '-P 6 2'
_symmetry_space_group_name_H-M   'P 6/m m m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            1
_cell_length_a                   3.036
_cell_length_b                   3.036
_cell_length_c                   3.098
_cell_volume                     24.730
_citation_journal_id_ASTM        PMANAI
_cod_data_source_file            boron_250.cif
_cod_data_source_block           B2Mn0.64Mo0.36
_cod_original_cell_volume        24.72952
_cod_database_code               1510755
Manganese boride, Mn B2
Bowan, A.L.; Nereson, N.G.; AIP Conference Proceedings 1974 (1974) 34–36; doi:

data_1510756
_publ_section_title
;
 Manganese boride, Mn B2
;
_journal_name_full               'AIP Conference Proceedings'
_journal_page_first              34
_journal_page_last               36
_journal_volume                  1974
_journal_year                    1974
_chemical_formula_sum            'B2 Mn'
_chemical_name_systematic        'Mn B2'
_space_group_IT_number           191
_symmetry_space_group_name_Hall  '-P 6 2'
_symmetry_space_group_name_H-M   'P 6/m m m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            1
_cell_length_a                   3.005
_cell_length_b                   3.005
_cell_length_c                   3.038
_cell_volume                     23.758
_citation_journal_id_ASTM        APCPCS
_cod_data_source_file            boron_251.cif
_cod_data_source_block           B2Mn1
_cod_original_cell_volume        23.75786
_cod_original_formula_sum        'B2 Mn1'
_cod_database_code               1510756
Zur Synthese und Kristallstruktur von Zinkboratoxiden mit isolierten, trigonal planaren BO3-Baugruppen: Zn5Mn(BO3)2O4 und ZnFe(BO3)O
Busche, S.; Bluhm, K.; Zeitschrift fuer Naturforschung, Teil B. Anorganische Chemie, Organische Chemie (42,1987-) 50 (1995) 1450–1454; doi:

data_7209438
_publ_section_title
;
 Zur Synthese und Kristallstruktur von Zinkboratoxiden mit isolierten,
 trigonal planaren BO3-Baugruppen: Zn5Mn(BO3)2O4 und ZnFe(BO3)O
;
_journal_name_full
;
Zeitschrift fuer Naturforschung, Teil B. Anorganische Chemie, Organische
 Chemie (42,1987-)
;
_journal_page_first              1450
_journal_page_last               1454
_journal_volume                  50
_journal_year                    1995
_chemical_formula_sum            'B2 Mn O10 Zn5'
_chemical_name_systematic        'Zn5 Mn (B O3)2 O4'
_space_group_IT_number           55
_symmetry_space_group_name_Hall  '-P 2 2ab'
_symmetry_space_group_name_H-M   'P b a m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   9.2641
_cell_length_b                   12.366
_cell_length_c                   3.0455
_cell_volume                     348.892
_citation_journal_id_ASTM        ZNBSEN
_cod_data_source_file            boron_252.cif
_cod_data_source_block           B2Mn1O10Zn5
_cod_original_cell_volume        348.8921
_cod_original_formula_sum        'B2 Mn1 O10 Zn5'
_cod_database_code               7209438
X-ray investigation of the rhenium-manganese-boron system
Telegus, V.S.; Kuz'ma, Yu.B.; Dopovidi Akademii Nauk Ukrains'koi RSR, Seriya A: Fiziko-Tekhnichni ta Matematichni Nauki 1969 (1969) 945–948; doi:

data_1510757
_publ_section_title
;
 X-ray investigation of the rhenium-manganese-boron system
;
_journal_name_full
;
Dopovidi Akademii Nauk Ukrains'koi RSR, Seriya A: Fiziko-Tekhnichni ta
 Matematichni Nauki
;
_journal_page_first              945
_journal_page_last               948
_journal_volume                  1969
_journal_year                    1969
_chemical_formula_sum            'B2 Mn Re3'
_chemical_name_systematic        'Mn Re3 B2'
_space_group_IT_number           70
_symmetry_space_group_name_Hall  'F 2 2 -1d'
_symmetry_space_group_name_H-M   'F d d d :1'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   7.832
_cell_length_b                   4.458
_cell_length_c                   15.38
_cell_volume                     536.994
_citation_journal_id_ASTM        DUKABM
_cod_data_source_file            boron_253.cif
_cod_data_source_block           B2Mn1Re3
_cod_original_cell_volume        536.9936
_cod_original_sg_symbol_Hall     '-F 2uv 2vw (x+1/8,y+1/8,z+1/8)'
_cod_original_formula_sum        'B2 Mn1 Re3'
_cod_database_code               1510757